OPEN

received: 21 October 2015 accepted: 17 February 2016 Published: 02 March 2016

Conduction Threshold in Accumulation-Mode InGaZnO Thin Film Transistors Sungsik Lee & Arokia Nathan The onset of inversion in the metal-oxide-semiconductor field-effect transistor (MOSFET) takes place when the surface potential is approximately twice the bulk potential. In contrast, the conduction threshold in accumulation mode transistors, such as the oxide thin film transistor (TFT), has remained ambiguous in view of the complex density of states distribution in the mobility gap. This paper quantitatively describes the conduction threshold of accumulation-mode InGaZnO TFTs as the transition of the Fermi level from deep to tail states, which can be defined as the juxtaposition of linear and exponential dependencies of the accumulated carrier density on energy. Indeed, this permits direct extraction and visualization of the threshold voltage in terms of the second derivative of the drain current with respect to gate voltage. Thin film transistors (TFTs) with disordered channel layers comprising say amorphous oxide or organic semiconductors, are becoming ubiquitous especially where low temperature processability and flexibility are essential1–3. To facilitate TFT systems design, a complete understanding on device physics and related device parameter extraction constitutes the first and inevitable step. In this vein, the work presented here on conduction threshold is a very fundamental device parameter. The work is applicable not only to thin film field effect transistor (FET) but also the pervasive silicon metal-oxide-semiconductor FET (MOSFET). Given its significance as a crucial indicator of carrier transport and instability in FETs4–10, the conduction threshold has to be determined physically rather than by empirical means11. Silicon MOSFETs conduct in inversion mode and the physical reason underlying the conduction threshold is well understood4,5. It corresponds to the critical state in which the induced or (inverted) carrier density becomes the same as the substrate’s majority carrier density5. For example, in an n-channel MOSFET, this transition point is when the electron density goes from linear to exponential dependence on energy in the solution of the Poisson-Boltzmann equation 5. This transition can be approximated empirically as the intercept made from a linear extrapolation on the drain current (IDS) vs. gate voltage (VGS) characteristic at very low drain voltage (VDS)5. In contrast to the silicon MOSFET, the TFT works in carrier accumulation mode regardless of the channel material6–9. This means that there is no polarity inversion of the induced carriers, so it is difficult to physically define the accumulation threshold. Moreover, because of the structural disorder of the semiconductor channel layer, there are localized deep and tail states distributed within the so-called band-gap, and depending on the position of the Fermi-level, free carriers or trapped carriers can be prevalent12,13. As a result, the conduction threshold is difficult to extract even empirically6,14–16. The density of carriers trapped at these localized states can be greater than free carriers, and there is no physical criteria for which all the traps are filled. In this family of devices, it is the localized trap states that determine the behaviour of field-effect mobility as a function of gate bias. In this letter, we present a systematic analysis of the conduction threshold leading to a physical definition of the threshold voltage in accumulation-mode InGaZnO TFTs. By solving the Poisson-Boltzmann equation coupled with measurements of the current-voltage characteristics, the total carrier density is captured as a function of the surface potential. Similar to the MOSFET, it turns out that there is a transition point in which the accumulated carrier concentration switches from a linear to an exponential dependence on energy, i.e. the free carrier density increases rapidly from this threshold level by virtue of trap-limited conduction. We find that this threshold can be directly extracted as the gate voltage in which the second derivative of IDS with respect to VGS peaks. This is visualized with the proposed grayscale image spectroscopy, allowing an ease of analysis on threshold voltage and related properties. The studies presented here show that the conduction threshold is independent of the band Electrical Engineering Division, Department of Engineering, University of Cambridge 9 JJ Thomson Avenue, Cambridge CB3 0FA, United Kingdom. Correspondence and requests for materials should be addressed to S.L. (email: [email protected]) or A.N. (email: [email protected])

Scientific Reports | 6:22567 | DOI: 10.1038/srep22567

1

www.nature.com/scientificreports/

Figure 1. (a) Photomicrograph and (b) schematic of the fabricated InGaZnO TFTs examined in this work. Measured drain current (IDS) vs. gate voltage (VGS) in (c) linear scale and (d) log scale, respectively. Here, we indicate an effective flat-band voltage ~0.3 V.

mobility and is largely determined by the sub-threshold characteristics associated with the deep states including interface states.

Results and Discussion

Microscopic conduction threshold. For the investigations reported here, we used a semiconducting oxide TFT test structure with a 50 nm thick InGaZnO channel layer, as seen in Fig. 1(a,b). The device is a typical bottom gate structure where Mo is used for electrodes. Here, the gate insulator is formed as a bilayer of SiOx and SiNx, and the total gate-insulator capacitance of this structure (Cox) is ~10 nF/cm2. As a final step, a single layer of SiOx is used for passivation layer and etch-stop layer (ESL). The TFT has a 50 μm channel width (W) and 10 μm channel length (L). Its IDS vs. VGS measured for VDS fixed at 10 mV is shown in Fig. 1(c,d). Here, we retrieve an effective flat-band voltage (VFB) of 0.3 V and a sub-threshold slope (SS) of 0.32 V/dec. Using the measured IDS − VGS characteristics, the microscopic picture in terms of free and trapped carrier densities can be captured as a function of VGS. The free charge density (Qfree) relates to the drain current as12,13, I DS = µb Q free (W /L) VDS.

(1)

where μb is the band mobility. Equation (1) is valid for both sub- and above-threshold regimes as long as VDS kT at T = 300 K. This confirms that the TLC is dominant at T = 300 K. Besides, the exponent (α ) in the power-law for the IDS − VGS curve above VT is defined as 2 kTt/kT – 1 for kTt > kT6,12,14,20. The value of α at T = 300 K is about 1.07 for kTt = 27 meV, which consistent with the observed linear dependence of IDS on VGS as seen in Fig. 1(c). As implied here, the role of Ntc and kTt is important in the TFT conduction, relating to the material composition. For example, with decreasing the ratio of In/Ga, field effect mobility of In-Ga-Zn-O TFTs can be reduced, suggesting a higher density of tail states (Ntc)21,22. In other words, if Ntc is higher, EF can be pinned at a lower energy from the conduction band minima (see Supplementary Information S6). This leads to a lower mobility reminiscent of the a-Si TFT whereas Fermi level in oxide TFT can even go into the conduction band due to its lower tail state density23. Based on the characteristic behaviour of the carrier densities shown in Fig. 2(c), the significance of the free carrier density (nfree) relative to the total carrier density (ntot = nfree + ndeep + ntail) can be defined as a ratio (χ TLC) in accordance to the TLC theory6,14,16, χTLC ≡

n free n free + ndeep + ntail

.

(9)

Using Equation (8) together with the values shown in Fig. 2(c), the behaviour of χ TLC and its first derivative with respect to VGS (i.e. ∂ χ TLC/∂ VGS) as a function of VGS is shown in Fig. 4(a,b), respectively. We see that ∂ χ TLC/∂ VGS peaks at VGS ~ 1.74 V regardless of the value of μb. This is consistent with our earlier observation of the common intercept seen in Fig. 2(c). Indeed, χ TLC shows a similarity with the first derivative of the current-voltage characteristics, ∂ IDS/∂ VGS, as seen in Fig. 4(a,c). As it turns out, ∂ IDS/∂ VGS is the trans- conductance of the transistor, which in turn is proportional to the field effect mobility (μFE). Thus, μFE is proportional to χ TLC. Indeed in accordance with the TLC theory, μFE can be defined as μb nfree/ntot = μb χ TLC6,20,24. At high VGS, Scientific Reports | 6:22567 | DOI: 10.1038/srep22567

5

www.nature.com/scientificreports/

Figure 4. (a) Trap-limited conduction (TLC) ratio (χ TLC) as a function of VGS. (b) The first derivative of χ TLC with respect to VGS. (c) The first derivative (i.e. ∂ IDS/∂ VGS) and (d) second derivative (i.e. ∂ 2IDS/∂ VGS2) of IDS vs. VGS. the behaviour of ∂ IDS/∂ VGS without effect of RC looks similar to χ TLC for μb = 20 cm2/V-s (see Supplementary Information S4). This suggests that μb of the examined device is ~20 cm2/V-s. The similarity between ∂ χ TLC/∂ VGS and the second derivative ∂ 2IDS/∂ VGS2 becomes even more striking in which the peak is at 1.74 V regardless of the band mobility (μb) values assumed for this analysis (see Fig. 4(b)). More importantly, the experimentally observed peak in ∂ 2IDS/∂ VGS2 vs. VGS appears at ~1.76 V which corroborates with theoretical prediction with a discrepancy less than 2%, as seen in Fig. 4(d). From the nature of the ∂ 2IDS/∂ VGS2 curve, we clearly identify the roles of deep and tail states, respectively, on either side of the peak where the threshold voltage lies. The deep states and corresponding sub-threshold slope determines the slope of the rising edge while the tail states and its exponent α are associated with that of the falling edge (see Fig. 4(d)).

Macroscopic observation of the threshold. The above analysis can be extended to measurements of device behaviour at different temperatures. Figure 5(a) shows IDS − VGS characteristics at T = 300 K, 200 K, 100 K, and the ∂ 2IDS/∂ VGS2 in each case is shown in Fig. 5(b). As the ambient temperature decreases, we observe that VT shifts to more positive VGS values. This is because of reduced thermal activation12. As temperature decreases, the current-voltage characteristic approaches a more power-law behaviour, as indicated in Fig. 5(a). Consequently, its second derivative converges to a non-zero value for VGS > VT, and which increases with decreasing temperature, as seen in Fig. 5(b). This is mainly associated with the tail state exponent (i.e. α = 2 kTt/kT–1), which increases with decreasing temperature. In contrast, the rising edge becomes increasingly steeper at lower temperatures, as indicated in Fig. 5(b). This is mainly due to the smaller sub-threshold slope (SS) at lower temperatures, which is typical of field effect transistors and can be intuitively explained with the relation, SS = ln(10)·kT/q(1 + Cdeep/ Cox)17, assuming Cdeep is independent of temperature. Scientific Reports | 6:22567 | DOI: 10.1038/srep22567

6

www.nature.com/scientificreports/

Figure 5. (a) Measured IDS vs. VGS for three different temperatures (T = 300 K, 200 K, and 100 K). (b) Normalized ∂ 2IDS/∂ VGS2 for different temperatures. (c) Three curves of IDS vs. VGS measured before and after + 20 V positive bias stress (PBS) for 500s and 1000s, respectively. (d) Normalized ∂ 2IDS/∂ VGS2 for different bias stress times. Note that each ∂ 2IDS/∂ VGS2 has been normalized to its peak value.

Figure 6. Grayscale images constructed from ∂ 2IDS/∂ VGS2 (a) for different temperatures, and (b) for different stress durations, respectively.

The observations of the current-voltage characteristics and its second derivative presented hitherto considerably simplify the interpretation of the shift in threshold voltage in bias stress experiments. More importantly, the shift in VT can be retrieved with minimizing an interruption to the stress measurement conditions. Figure 5(c) shows the measured IDS − VGS characteristics following positive bias stress (i.e. PBS at VGS = + 20 V while maintaining VDS = 0 V) for stress durations (tPBS) of 500 sec and 1000 sec. As seen in Fig. 5(d), there is a positive VT-shift, which increases with stress duration. Since the value of ∂ 2IDS/∂ VGS2 in a well-above VT regime Scientific Reports | 6:22567 | DOI: 10.1038/srep22567

7

www.nature.com/scientificreports/ remains zero for all cases, as seen in Fig. 5(d), it suggests that there is no significant degradation in band tail states (e.g. kTt), thus unaffecting the tail state exponent α . This suggests electron trapping into the gate insulator as the significant and likely source of VT-shift. However, the ∂ 2IDS/∂ VGS2 curve appears to spread out more for longer tPBS. Indeed, the slope of the rising edge (at VGS